Lithium Chalcogenidotetrelates: LiChT—Synthesis and Characterization of New Li+Ion Conducting Li/Sn/Se Compounds
Kaib, Thomas; Bron, Philipp; Haddadpour, Sima; Mayrhofer, Leonhard; Pastewka, Lars; Järvi, Tommi T.; Moseler, Michael; Roling, Bernhard; Dehnen, Stefanie; Chemistry of Materials 25 (2013) 2961–; doi:10.1021/cm400541n

data_4001781
_publ_section_title
;
 Lithium Chalcogenidotetrelates: LiChT---Synthesis and Characterization of
 New Li+Ion Conducting Li/Sn/Se Compounds
;
_journal_issue                   15
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2961
_journal_paper_doi               10.1021/cm400541n
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'Li4 Se4 Sn'
_chemical_formula_weight         462.29
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4
_audit_creation_date             2010-06-11T16:40:56-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.931(3)
_cell_length_b                   8.2217(16)
_cell_length_c                   6.5989(13)
_cell_measurement_temperature    173(2)
_cell_volume                     810.1(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.796
_diffrn_measured_fraction_theta_max 0.796
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1188
_diffrn_reflns_av_unetI/netI     0.0617
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            1826
_diffrn_reflns_theta_full        26
_diffrn_reflns_theta_max         26
_diffrn_reflns_theta_min         4.81
_exptl_absorpt_coefficient_mu    21.016
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    3.791
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'cut needle'
_exptl_crystal_F_000             792
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.15
_refine_diff_density_max         2.011
_refine_diff_density_min         -2.119
_refine_diff_density_rms         0.388
_refine_ls_extinction_coef       0.0044(12)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.13
_refine_ls_matrix_type           full
_refine_ls_number_parameters     45
_refine_ls_number_reflns         683
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.13
_refine_ls_R_factor_all          0.0517
_refine_ls_R_factor_gt           0.049
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0926P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1367
_refine_ls_wR_factor_ref         0.139
_reflns_number_gt                639
_reflns_number_total             683
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            cm400541n_si_002.cif
_cod_data_source_block           1
_cod_original_cell_volume        810.0(3)
_cod_database_code               4001781